Dilithium (citrate) crystals and their relatives.
Cigler, Andrew J.; Kaduk, James A.; Acta crystallographica. Section C, Structural chemistry 74 (2018) 1160–1170; doi:10.1107/S2053229618012597

data_2311995
_publ_section_title
;
 Dilithium (citrate) crystals and their relatives.
;
_journal_issue                   'Pt 10'
_journal_name_full
'Acta crystallographica. Section C, Structural chemistry'
_journal_page_first              1160
_journal_page_last               1170
_journal_paper_doi               10.1107/S2053229618012597
_journal_volume                  74
_journal_year                    2018
_chemical_formula_analytical     'C6 H6 Li Na O7'
_chemical_formula_moiety         'Li Na H C6 H5 O7'
_chemical_formula_structural     'Li Na H C6 H5 O7'
_chemical_formula_sum            'C6 H6 Li Na O7'
_chemical_formula_weight         220.04
_chemical_name_common            'lithium sodium hydrogen citrate'
_chemical_name_systematic        'lithium sodium hydrogen citrate'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_audit_creation_date             2017-04-21T13:32
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
;
2017-04-21T13:32  Initial CIF as created by GSAS2CIF

2017-05-16 # Formatted by publCIF
;
_cell_angle_alpha                91.762(5)
_cell_angle_beta                 104.388(5)
_cell_angle_gamma                97.438(4)
_cell_formula_units_Z            2
_cell_length_a                   6.5811(4)
_cell_length_b                   6.3570(4)
_cell_length_c                   9.9389(5)
_cell_measurement_temperature    300
_cell_volume                     398.52(4)
_computing_structure_refinement  GSAS
_computing_structure_solution    FOX
_diffrn_ambient_temperature      300
_diffrn_detector                 'Si strip'
_diffrn_detector_type            Xcelerator
_diffrn_measurement_device_type  'PANalytical Empyrean'
_diffrn_radiation_polarisn_ratio 0.5
_diffrn_radiation_probe          x-ray
_diffrn_source                   'sealed X-ray tube'
_diffrn_source_target            Mo
_diffrn_source_type              'PANalytical Empyrean'
_exptl_absorpt_coefficient_mu    0.073
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  1.00000
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 No correction is applied.
;
_exptl_crystal_density_diffrn    1.834
_pd_block_id                     2017-04-21T13:32|KADU1688|James_A._Kaduk|nccpan
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  white
_pd_instr_dist_spec/detc         240
_pd_instr_dist_src/spec          240
_pd_meas_2theta_range_inc        0.01671
_pd_meas_2theta_range_max        49.99084
_pd_meas_2theta_range_min        1.0109
_pd_meas_number_of_points        2932
_pd_meas_scan_method             step
_pd_phase_name                   'Li Na H C6 H5 O7'
_pd_prep_temperature             393
_pd_proc_2theta_range_inc        0.01671
_pd_proc_2theta_range_max        49.99084
_pd_proc_2theta_range_min        1.0109
_pd_proc_info_datetime           2017-04-21T13:32:20
_pd_proc_ls_background_function
;   GSAS Background function number 1 with  1 terms.
 Shifted Chebyshev function of 1st kind
      1:    771.559    
;
_pd_proc_ls_peak_cutoff          0.01000
_pd_proc_ls_profile_function
;
 CW Profile function number 4 with  27 terms
 Pseudovoigt profile coefficients as parameterized in
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 Asymmetry correction of L.W. Finger, D.E. Cox & A. P. Jephcoat (1994).
 J. Appl. Cryst.,27,892-900.
 Microstrain broadening by P.W. Stephens,  (1999). J. Appl. Cryst.,32,281-289.
 #1(GU)   =  186.900 #2(GV)   =    0.000 #3(GW)   =    0.100
 #4(GP)   =    0.000 #5(LX)   =    0.989 #6(ptec) =     0.00
 #7(trns) =     0.00 #8(shft) =   0.0000 #9(sfec) =     0.00
 #10(S/L) =   0.0159 #11(H/L) =   0.0160 #12(eta) =   0.6917
 Peak tails are ignored  where the intensity is below 0.0100 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0347
_pd_proc_ls_prof_wR_expected     0.0231
_pd_proc_ls_prof_wR_factor       0.0439
_pd_proc_number_of_points        2932
_pd_spec_mounting                'Glass capillary'
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_pd_spec_size_axial              12
_pd_spec_size_equat              1
_pd_spec_size_thick              1
_refine_ls_goodness_of_fit_all   2.05
_refine_ls_hydrogen_treatment    refU
_refine_ls_matrix_type           full
_refine_ls_number_parameters     64
_refine_ls_number_restraints     29
_refine_ls_R_Fsqd_factor         0.14161
_refine_ls_shift/su_max          0.03
_refine_ls_shift/su_mean         0.01
_refine_ls_weighting_scheme      sigma
_reflns_d_resolution_high        0.839
_reflns_d_resolution_low         9.607
_reflns_limit_h_max              7
_reflns_limit_h_min              0
_reflns_limit_k_max              7
_reflns_limit_k_min              -7
_reflns_limit_l_max              11
_reflns_limit_l_min              -11
_reflns_number_total             2806
_cod_data_source_file            ov3116sup4.cif
_cod_data_source_block           KADU1688_publ
_cod_original_cell_volume        398.519(23)
_cod_database_code               2311995
_publcif_datablock.id            {ad0b0c3f-1930-4201-8fb7-98c66b649f4f}
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n